# A “Non-Invasive” Technique for Qualifying the Reinforced Concrete Structure

Authors: Antonella Guida; Antonello Pagliuca; Alessandro Tranquillino Minerva
Journal: International Journal of Geophysics
 (2012)

---

## Abstract

In recent years, a lot of studies on built heritage emphasize the need to use appropriate techniques to evaluate the current condition of the structure before designing an intervention. The research focuses on the restoration of reinforced concrete buildings that begin to show signs of decay and deterioration. To verify the state of a building, it’s possible to use the “destructive” methods (that require a local removal of material) and “nondestructive” tests. The combined results from different “nondestructive” tests are very interesting instruments to assess the concrete strength. This methodological approach can help to reduce the possible errors when using the sclerometer and ultrasonic tests separately; in this way, the combined method called “SonReb” (SONic + REBound) was developed. This paper would highlight the importance with respect to cultural heritage buildings and on the studied structure and contribute to developed engineering strategies to maintenance and restoration. The above-defined methodology has been tested on a postwar building which is located in Gravina in Puglia (Italy): the “Centrone” theatre; it was built using a mixed structure, that is, reinforced concrete and bearing masonry built of local stone. The building was used until the 1990s and now is abandoned. The analysis and qualification of the masonry structures of built heritage show how this approach is useful for classifying the pathological events on each building and to implement the innovative solutions to improve the durability of a restoration intervention.


---

## Body

## 1. Introduction

In the last decades, the architectural heritage of the modern movement seems to be more at risk than during any other period. This built inheritance embodies the dynamic spirit of the industrial age. At the end of the 1980s, many modern masterpieces had already been demolished or changed beyond recognition. This was mainly due to the fact that many were not considered to be elements of heritage that their original functions have substantially changed and that their technological innovations have not always endured long-term stresses.A thorough research of built heritage enables understanding of the evolution of design philosophies and underlying cultural meanings and messages, artistic and functional qualities, and engineering achievements. A detailed knowledge of building materials, construction techniques, environmental services, external impacts, and internal impacts of use or disuse assist in identifying the problems affecting buildings and defining a methodological approach for interventions.The research objective is to provide new qualitative information on the strength of reinforced concrete structures of a building by using innovative, non-invasive testing techniques. The case of study is the“Centrone” theatre in Gravina in Puglia (Italy).The confluence of the local architectural styles (vernacular and academic) and the emerging aesthetic of reinforced concrete is explored to outline the context that influenced the building design.The research methodology includes (a) the context in which the buildings were designed, (b) their history, (c) building technologies used, (d) non-invasive testing of the reinforced concrete structures, (e) the analysis of the test results, and (f) the conclusions.Testing methods could be “destructive”, as they require a local removal of material, or “nondestructive”, that is, they do not affect the structure. A sclerometer test, an ultrasonic test and their combined use, called SonReb(SONic + REBound), are “nondestructive” tests on reinforced concrete. The combined tests are a very useful method for assessing the concrete strength and to reduce the possibility of errors that can happen if the tests are not combined, as it has been noticed that the humidity content of a structural element can influence the sclerometer index and the ultrasound speed [1]. The combined method requires shorter time to obtain the results.


## 2. A“Critical” Approach to Building Restoration

The conservation intervention on a historic building, regardless of its architectural and/or artistic value, is generally more appropriate if information on its construction, evolution to date, materials, construction techniques, and structure is available. The conservation of built heritage highlights different issues such as the vast number of buildings needing attention and the urgency of cases that have to be resolved with limited economic resources and time.To undertake a suitable intervention, three questions have to be answered: whether, where, and how to restore. The fourth question could be added, in which the economic aspect dominates: when to restore. To be able to respond adequately to these questions, it is necessary to proceed by developing specifications step by step, starting from a detailed knowledge of the entire building, the level and causes of degradation, and by finishing with the “operational” description of the proposed interventions.Within the preliminary data acquisition phase, the direct survey of the building characteristics and condition and the mapping of any noticed changes are accompanied by the research on the project documentation and the events that have affected the structure during its construction and throughout the building life.These approaches, often coupled with normative models which translate living conditions into objective parameters and standards, hinder the interventions such as a “simple” maintenance or a restoration or produce the result that is not logically related to the structural, typological, functional, and technological characteristics of the artefacts.An “appropriate” restoration should plan the reuse of built heritage and aim to achieve building performance comparable to new buildings. The reuse interventions should be integrated with the conservation and not imposed.The above methodology highlights how the approach could be helpful for the classification of pathological events within a building and for the application of innovative solutions to increase the durability of restoration interventions.


## 3. The Investigative Techniques for Concrete

The investigative techniques for concrete are also classified in two defined macrocategories (“destructive” and “nondestructive”). The former are based on the extraction of concrete samples to undertake compressive tests and represent the most reliable instrument for assessing the mechanical properties of concrete. The second investigative typology, the nondestructive tests, can be further subdivided in: really “nondestructive” investigations and “partially destructive” investigations. The latter include (a) the penetration test with a Windsor gun (ASTM C 83) which enables the identification of compressive resistance of concrete by measuring the depth of penetration of the special metal pins projected with a Windsor gun into concrete, (b) the extraction test (pull-out) (UNI 10157 : 1992-ASTM C 900-06) which enables the assessment of compressive resistance of concrete by measuring the force used by a hydraulic jack for extracting a special plug inserted into concrete.The really nondestructive investigations include, among others, (a) endoscopy that enables a direct observation of form and appearance of an investigated object, (b) thermography that assists in recognising potential structural anomalies by using the capacity of materials to transfer heat, (c) magnetometry which enables localising metal bars in reinforced concrete, (d) the Ground Penetrating Radar (GPR), especially with regard the investigation of the internal reinforcement bars, (e) measurement of the electric potential of concrete which enables defining the level of corrosion of metal reinforcements in concrete, (f) ultrasound investigation that allows qualitative assessment of the concrete resistance by using the capacity of the concrete components to transfer ultrasound waves, (g) sclerometric tests that assess the concrete resistance by reading the bounce results, and finally, (h) so-called “SonReb” (SONic + REBound) that enables assessing the concrete resistance by combining the speed of ultrasound waves and the index of surface bounce through a synergic use of the two previous investigations.


### 3.1. The“SonReb” Method for Determining the Resistance of Concrete

The SonReb method, as mentioned above, allows a qualitative determination of the concrete resistance [2] through the cross-examination of the values of the speed of ultrasound waves and the values of sclerometric bounce. This investigation method is standardised by RILEM Recommendations [3] 43 CND-EN 13791 : 2007, the EC regulation 1-2010 UNI EN 12504-2 : 2001, ASTM C597, UNI EN 12504-4 : 2005, the Test Report CUR 69, the standards UNI 7997, UNI 9524 and UNI 83308.This method is used for assessing the resistance of concrete, enabling the elimination of errors, at least partly, that appear when the two investigation methods are separately applied. This method, in fact, allows reducing the errors made when the sclerometric and ultrasound tests are undertaken separately [4].It has been noticed, for example, that the humidity content leads to an underestimation of the sclerometric index and in an inversely proportional way leads to an overestimation of the ultrasound speed; similarly, the sclerometric index rises in a directly proportional way to the increase of the age of concrete [1], while the ultrasound speed decreases in an inversely proportional way to it [5].In fact, the risk that can come up in the separate use of sclerometric and/or ultrasound tests is related, for example, to the chance nature of the position of aggregates in relation to the external surface of an investigated component; the sclerometer can easily beat against a large piece of aggregate, probably obtaining a higher value of the bounce index S in relation to the one returned when the blow is executed on a homogenous concrete surface (Figure1).Figure 1
Sclerometer beats against a large piece of aggregate.Again as an example, the ultrasound test (Figure2) can equally be affected by the chance nature of the disposition of aggregates in a cement mix when the gaps between the aggregates are arranged in the way that induces the rise of the void index; in this case, the speed of wave spread V decreases in relation to the value that would be obtained when the wave spreads through an area of “homogenous” concrete.Figure 2
Ultrasound equipment: the impulse transmission.The application of the “SonReb” method asks for the appraisal [6] of local values of the ultrasound speed V and of the bounce index S from which it is possible to obtain the resistance of concrete Rc through expressions such as:
(a)Rc,sonReb=a·Sb·Vc.
In the scientific literature this formula has assumed different forms, each one expressing the experiments undertaken directly on site or in a laboratory on standardised samples.For example:(i)
Gasparik [7] (1992)
(b)Rc,2=8,06·10-8·S1,246·V1,85,(ii)
RILEM (1993) [2], NDT 4
(c)Rc,1=9,27·10-11·S1,4·V2,6,(iii)
Di Leo and Pascale [6] (1994)
(d)Rc,3=1,2·10-9·S1,058·V2,446,in which:(i)
Rc is the resistance of a cube under compression [N/mm2];(ii)
S is the sclerometric index;(iii)
V is the ultrasound speed [m/s].The formula(c) depicts the correlation curve applied in the investigated case studies. In (c)  Rc is expressed in MPa and the ultrasound speed in m/s; this relationship is related to a standard concrete whose properties are described in RILEM 43-CND. When a different type of concrete is employed the following relationship is applicable [8]:
(1)RsonReb=RsonReb′·(Cc·Cd·Ca·Cf·CP·Cm),
where RsonReb′ is the value obtained from (1), while Cc (cement type), Cd (cement content), Ca (aggregate types), Cf (proportions of fines), Cp (maximum aggregate size), and Cm (errors) are coefficients of influence that permit the extension of (b) to the cases of a nonstandard concrete (as defined above).Hence, if the concrete has the same characteristics as the one whose experimental curves are available, the graph directly provides the estimated resistance of concrete. Otherwise, as usually happens, when the concrete has a different composition from the one presented by the curve, the corrective coefficients, that take into account the type of cement and the related dosage, the nature and dimensions of aggregates, and the potential additives need to be applied to obtain an approximately true estimate of the concrete resistance [1].It is evident that the above equations could not have universal validity except for the fact that the values ofS and V depend on the characteristics of concrete, even when the specific indications on the limitations of applicability are missing.However, a qualitative appraisal of the resistance of concrete can be made even by using the graphs (Figure3) which show a series of isoresistance curves in the plane V-S (obtained from the above analytic expressions) and which refer to the tests undertaken on standardised samples in a laboratory.Figure 3
Example of isoresistance curves—RILEM NDT 4 recommendations.Although it appears absolutely necessary to analyse a wider range of cases, the above methodological investigation approach, based on the comparative analysis of the two described test campaigns, suggests several important considerations regarding the modality of investigation and the interpretation of results, demonstrating the need for establishing general investigation criteria: more than defining in a strict manner the number of tests that should be undertaken, it would be necessary to preset the level of significance to be achieved.


## 3.1. The“SonReb” Method for Determining the Resistance of Concrete

The SonReb method, as mentioned above, allows a qualitative determination of the concrete resistance [2] through the cross-examination of the values of the speed of ultrasound waves and the values of sclerometric bounce. This investigation method is standardised by RILEM Recommendations [3] 43 CND-EN 13791 : 2007, the EC regulation 1-2010 UNI EN 12504-2 : 2001, ASTM C597, UNI EN 12504-4 : 2005, the Test Report CUR 69, the standards UNI 7997, UNI 9524 and UNI 83308.This method is used for assessing the resistance of concrete, enabling the elimination of errors, at least partly, that appear when the two investigation methods are separately applied. This method, in fact, allows reducing the errors made when the sclerometric and ultrasound tests are undertaken separately [4].It has been noticed, for example, that the humidity content leads to an underestimation of the sclerometric index and in an inversely proportional way leads to an overestimation of the ultrasound speed; similarly, the sclerometric index rises in a directly proportional way to the increase of the age of concrete [1], while the ultrasound speed decreases in an inversely proportional way to it [5].In fact, the risk that can come up in the separate use of sclerometric and/or ultrasound tests is related, for example, to the chance nature of the position of aggregates in relation to the external surface of an investigated component; the sclerometer can easily beat against a large piece of aggregate, probably obtaining a higher value of the bounce index S in relation to the one returned when the blow is executed on a homogenous concrete surface (Figure1).Figure 1
Sclerometer beats against a large piece of aggregate.Again as an example, the ultrasound test (Figure2) can equally be affected by the chance nature of the disposition of aggregates in a cement mix when the gaps between the aggregates are arranged in the way that induces the rise of the void index; in this case, the speed of wave spread V decreases in relation to the value that would be obtained when the wave spreads through an area of “homogenous” concrete.Figure 2
Ultrasound equipment: the impulse transmission.The application of the “SonReb” method asks for the appraisal [6] of local values of the ultrasound speed V and of the bounce index S from which it is possible to obtain the resistance of concrete Rc through expressions such as:
(a)Rc,sonReb=a·Sb·Vc.
In the scientific literature this formula has assumed different forms, each one expressing the experiments undertaken directly on site or in a laboratory on standardised samples.For example:(i)
Gasparik [7] (1992)
(b)Rc,2=8,06·10-8·S1,246·V1,85,(ii)
RILEM (1993) [2], NDT 4
(c)Rc,1=9,27·10-11·S1,4·V2,6,(iii)
Di Leo and Pascale [6] (1994)
(d)Rc,3=1,2·10-9·S1,058·V2,446,in which:(i)
Rc is the resistance of a cube under compression [N/mm2];(ii)
S is the sclerometric index;(iii)
V is the ultrasound speed [m/s].The formula(c) depicts the correlation curve applied in the investigated case studies. In (c)  Rc is expressed in MPa and the ultrasound speed in m/s; this relationship is related to a standard concrete whose properties are described in RILEM 43-CND. When a different type of concrete is employed the following relationship is applicable [8]:
(1)RsonReb=RsonReb′·(Cc·Cd·Ca·Cf·CP·Cm),
where RsonReb′ is the value obtained from (1), while Cc (cement type), Cd (cement content), Ca (aggregate types), Cf (proportions of fines), Cp (maximum aggregate size), and Cm (errors) are coefficients of influence that permit the extension of (b) to the cases of a nonstandard concrete (as defined above).Hence, if the concrete has the same characteristics as the one whose experimental curves are available, the graph directly provides the estimated resistance of concrete. Otherwise, as usually happens, when the concrete has a different composition from the one presented by the curve, the corrective coefficients, that take into account the type of cement and the related dosage, the nature and dimensions of aggregates, and the potential additives need to be applied to obtain an approximately true estimate of the concrete resistance [1].It is evident that the above equations could not have universal validity except for the fact that the values ofS and V depend on the characteristics of concrete, even when the specific indications on the limitations of applicability are missing.However, a qualitative appraisal of the resistance of concrete can be made even by using the graphs (Figure3) which show a series of isoresistance curves in the plane V-S (obtained from the above analytic expressions) and which refer to the tests undertaken on standardised samples in a laboratory.Figure 3
Example of isoresistance curves—RILEM NDT 4 recommendations.Although it appears absolutely necessary to analyse a wider range of cases, the above methodological investigation approach, based on the comparative analysis of the two described test campaigns, suggests several important considerations regarding the modality of investigation and the interpretation of results, demonstrating the need for establishing general investigation criteria: more than defining in a strict manner the number of tests that should be undertaken, it would be necessary to preset the level of significance to be achieved.


## 4. The Case of Study: “Centrone” Theatre in Gravina in Puglia (Italy)

The above-defined methodology has been tested on a postwar building which is located in Gravina in Puglia (Italy): the “Centrone” theatre; it was built using a mixed structure, that is, reinforced concrete and bearing masonry built of local stone.The building is not very old, but it is very interesting for the local civic history; in fact, it represents different values. Values that are set in different reels from the life of the building and revolved the surrounding environment in which it is inserted.Historical value related to the historical development of the building and to the importance that it has in terms of expression of the local civic history; social value that is related to the social development of the city; cultural value that is related to the cultural growth of society; value of identity that has the building in terms of physics and metaphysics belong to a place then; but not least; the economic value related to the ability to reuse the building readapting it to new needs.The building was built between 1946 and 1948; the foundations were built on pillars and vaults (Figure4) and the pitched roof using iron trusses (Figure 5).Figure 4
Historical image of vault construction.Figure 5
Historical image of iron trusses.The building is a rectangular block (Figure6), developed on three levels and covered using plaster and stone; the main façade is symmetrical, tripartite and follows the ground inclination; in the opposite side, the building shows two projecting polygonal elements realized using the local stone.Figure 6
The “Centrone” theatre in Gravina in Puglia (Italy).In the central part of the building; approximately 10 m wide; is located the entrance, highlighted by the massive presence of two Doric columns that support a loggia. The building is organized in different spaces: the central part, where at ground floor there are the foyer entrance and ticket office, while on the first floor there is the Room “Italy” (Figure7) that contains 110 seats; at second floor there are three flats for the managers of the theatre. The mail hall contains the stalls with 800 seats (a big space 32.5 m long and 21 m wide); it is partly covered by a balcony (at the first level) with 300 seats and a gallery on the second level with 300 seats.Figure 7
The room “Italy” on the first floor of the theatre.The pathologies that interest the building are not particularly serious, since it does not affect in any way the static system of structure and are easily solvable with non-invasive interventions. Inside are not detectable serious and manifest diseases, except for some water infiltrations from the roof that are determined as chromatic alterations and plaster detachment.The condition of the pillars is generally acceptable, since they do not show obvious pathologies; however, you should note that some have a bad state of preservation of the plaster due to moisture that caused severe swelling, internal cavities and an evident surface lack of homogeneity.


### 4.1. On-Site Tests: Formulation

Essential elements for the organisation of an investigation campaign are the selection of the components that will be examined (which have to be representative of the whole structure), the investigation methodology that will be used, and the number and location of the investigation points; these requirements, in fact, are fundamental to guarantee a certain level of “reliability” of the obtained results and a “trustworthiness” with regard to the qualitative indications related to the characteristics of the material. In the case of the “Centrone” theatre, the identification of the components to be investigated was made by selecting the structural components which make the internal core of the load-bearing structure for two reasons: (1) because they enable to investigate a concrete in the state of “natural aging” (i.e., without considering the aggressive atmospheric agents which could have modified the condition of the material) and (2) for easiness of selecting the testing points. The structure of the whole building consists of a dual typology of structural components: those inserted in the external fabric (therefore difficult to investigate) and those located within the building.The selection of the location of the investigation points (Figure8) was random (with the aim to guarantee the representativeness of the investigation for the entire structure); in addition, “homogenous” areas [1] (which have the same characteristics) were noted and considered by making the obtained results “qualitative” and representative for all the components that show the same characteristics; a further condition is that the selected surfaces do not show any obvious condition of degradation. The methodology used to undertake the tests was exclusively selected in terms of the possibility to undertake the tests. Regarding the sclerometric tests, they were undertaken by placing the instrument always orthogonally in relation to the investigated surface; the preference was given to the direct method of investigation.The considered reference (in terms of the number of tests with the aim to guarantee the reliability of the results) for the investigation campaign was taken from the framework of the Italian investigation procedures.Figure 8
The specification of the location of the investigation points.


### 4.2. On-Site Tests: Analysis and Results

Sclerometer tests were carried out following the directions contained in UNI EN 12504-2 (2001). The instrument used is the concrete GEI model. On each pillar identified, it was carried out 10 measurements (Table1) of the value of rebound (for each test, ten values were taken, from which the average value was considered as illustrative).Table 1
The value of rebound index.
Structural element
Sclerometer value
Average value
Element code
Size [cm]
Rebound value
P1 Dx  T
43 × 43
27
28
26
29
25
25
31
26
28
28
28
P2 Dx   T
43 × 43
34
38
36
42
40
36
37
38
41
38
38
P3 Dx   T
43 × 43
32
33
30
31
32
32
34
31
31
31
32
P4 Dx   T
43 × 43
35
33
34
30
36
34
34
34
36
38
38
P5 Dx   T
43 × 43
35
33
34
34
33
32
35
37
34
34
34
P6 Dx   T
43 × 43
35
37
38
38
36
34
35
38
36
36
36
P1 Sx  T
43 × 43
41
37
45
47
37
38
42
39
40
41
41
P2 Sx  T
43 × 43
43
42
42
40
44
42
46
44
44
40
43
P3 Sx  T
43 × 43
34
34
37
35
34
33
34
32
36
35
34
P4 Sx T
43 × 43
32
28
32
32
34
34
34
34
30
32
32
P5 Sx   T
43 × 43
30
28
28
32
30
28
32
32
30
30
30
P6 Sx  T
43 × 43
34
35
34
36
35
37
38
35
38
35
36
P1 Dx   I p
43 × 43
23
21
21
22
22
25
25
26
24
22
23
P2 Dx   I p
43 × 43
33
32
33
32
30
30
30
33
31
30
31
P3 Dx  I p
43 × 43
37
40
38
41
43
38
38
38
41
38
39
P4 Dx   I p
43 × 43
38
38
38
38
37
39
37
38
39
39
38
P5 Dx   I p
43 × 43
37
39
35
38
37
38
38
40
38
40
38
P6 Dx   I p
43 × 43
36
38
37
37
38
38
37
38
36
38
37
P1 Sx  I p
43 × 43
26
22
24
22
24
20
23
22
22
22
23
P2 Sx  I p
43 × 43
40
41
37
40
40
39
38
38
37
38
39
P3 Sx  I p
43 × 43
40
37
35
37
36
35
35
35
35
35
36
P4 Sx  I p
43 × 43
35
35
35
37
35
37
36
38
36
38
36
P5 Sx  I p
43 × 43
40
40
37
35
36
35
38
36
36
36
37
P6 Sx  I p
43 × 43
36
38
36
38
38
38
40
40
38
38
38Three different areas were selected for each investigated component; at 0.70 m, at 1.40 m, and at 2.10 m from the floor. This selection, in fact, was motivated by the need to investigate the columns at the points of major stress (base and middle), having assumed (1) a uniform distribution of the loads and imposed loads (due to the homogenous structure) and (2) a homogenous condition of the loads (there are no visible cracks to induce any different considerations).Ultrasonic tests were carried out according to the UNI EN 12504-4 (2005). Ultrasonic equipment used is the DSP model of Ultrasonic UTD 1004. On each pillar identified, it was carried out 10 measurements (Table2) of the value of rebound (for each test ten values were taken, from which the average value was considered as illustrative).Table 2
The value of ultrasonic speed.
P1 Sx T average ultrasonic speed: 2862,9 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2039
2036
2035
2038
2041
2032
2034
2045
2048
2029
Y direction
3656
3669
3686
3676
3664
3668
3672
3675
3663
3665
Height: 1,40 mSize 0,43 × 0,43
X direction
2043
2041
2042
2045
2046
2049
2068
2061
2043
2048
Y direction
3665
3681
3687
3690
3684
3689
3676
3679
3695
3700
Height: 2,10 mSize 0,40 × 0,40
X direction
2052
2045
2049
2046
2048
2058
2060
2039
2059
2056
Y direction
3685
3684
3682
3679
3669
3689
3694
3692
3686
3696
P1 Dx  T average ultrasonic speed: 2873,2 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
3367
3355
3362
3360
3355
3394
3397
3389
3362
3392
Y direction
2520
2521
2531
2513
2512
2515
2510
2533
2511
2525
Height: 1,40 mSize 0,43 × 0,43
X direction
3250
3257
3260
3252
3247
3302
3315
3333
3341
3348
Y direction
2490
2499
2510
2512
2505
2496
2493
2495
2491
2510
Height: 2,10 mSize 0,40 × 0,40
X direction
3322
3320
3333
3327
3325
3139
3152
3134
3152
3157
Y direction
2526
2516
2545
2544
2558
2556
2559
2562
2568
2564
P6 Sx  T average ultrasonic speed: 2134,1 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2160
2084
2053
2016
2066
2161
2016
2103
2105
2150
Y direction
2160
2154
2111
2102
2013
2163
2136
2165
2130
2122
Height: 1,40 mSize 0,43 × 0,43
X direction
2160
2136
2165
2154
2155
2155
2153
2151
2160
2165
Y direction
2152
2154
2150
2153
2103
2100
2155
2015
2140
2150
Height: 2,10 mSize 0,40 × 0,40
X direction
2150
2099
2088
2066
2200
2035
2150
2156
2171
2015
Y direction
2030
2105
2145
2144
2014
2156
2148
2154
2148
2154
P6 Dx  T average ultrasonic speed: 2560,9 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2562
2563
2545
2568
2567
2575
2574
2586
2544
2578
Y direction
2543
2546
2566
2564
2568
2545
2544
2543
2549
2548
Height: 1,40 mSize 0,43 × 0,43
X direction
2566
2531
2533
2540
2545
2562
2545
2565
2555
2551
Y direction
2556
2565
2559
2557
2549
2552
2553
2545
2551
2553
Height: 2,10 mSize 0,40 × 0,40
X direction
2565
2596
2586
2567
2568
2564
2572
2575
2574
2573
Y direction
2564
2561
2563
2559
2568
2567
2586
2584
2583
2569
P1 Sx  I p average ultrasonic speed: 2582,0 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
1899
2130
2156
2102
2105
2111
2182
2221
2310
2229
Y direction
3200
3180
3196
3102
3104
3016
3038
3086
3048
3062
Height: 1,40 mSize 0,43 × 0,43
X direction
1700
1750
1890
1806
1830
1834
1905
1942
1972
1973
Y direction
3109
3140
3149
3131
3158
3160
3263
3264
3285
3189
Height: 2,10 mSize 0,40 × 0,40
X direction
2005
2103
1999
2150
2015
2060
2160
2163
2184
2150
Y direction
3005
3158
3139
3190
3100
3089
3048
3069
3099
3105
P1 Dx  I p average ultrasonic speed: 3006,5 m/s
Height: 0,70 mSize 0,46 ×  0,46
X direction
3000
3002
3005
3019
2993
3010
3015
3019
2921
2996
Y direction
3012
3015
3018
3016
3018
3001
3021
3029
3028
3020
Height: 1,40 mSize 0,43 ×  0,43
X direction
3000
3052
3013
3002
3015
2999
3050
3015
3016
3019
Y direction
2996
3047
3036
3033
3031
3002
3052
3035
3063
3043
Height: 2,10 mSize 0,40 ×  0,40
X direction
2899
2915
3005
3001
3045
3015
3062
3036
3035
3046
Y direction
3051
3015
3063
3026
3033
3018
3017
3021
3012
3026These data were compared with the method “SonReb” (Tables3, 4, 5, and 6) to improve—as said before—the qualitative interpretation of results; the analysis showed satisfactory results of the state of concrete condition, as well as the importance to compare the ultrasonic and sclerometer tests.Table 3
Left side pillar (Sx): Ground floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Sx T
41
2862,9
P2 Sx T
43
3297,1
P3 Sx T
34
3345,3
P4 Sx T
32
3181,2
P5 Sx T
30
3192,1
P6 Sx T
36
2134,1Table 4
Right side pillar (Dx): Ground floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Dx T
28
2873,2
P2 Dx T
38
3103,6
P3 Dx T
32
3199,3
P4 Dx T
38
3313,2
P5 Dx T
34
3082,1
P6 Dx T
36
2560,9Table 5
Left side pillar (Sx): First floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Sx I p
23
2582,0
P2 Sx I p
39
3476,1
P3 Sx I p
36
3358,2
P4 Sx I p
36
3319,6
P5 Sx I p
37
3450,3
P6 Sx I p
38
3346,1Table 6
Right side pillar (Dx): First floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Dx I p
23
3006,5
P2 Dx I p
31
3210,2
P3 Dx I p
39
3120,9
P4 Dx I p
38
3204,6
P5 Dx I p
38
3098,1
P6 Dx I p
37
3301,5The obtained results show a significant homogeneity of values measured at each investigated level; more precisely, the sclerometric tests show an average value (of the ten measurements made at each point) of the bounce index uniformly distributed on the surfaces; whereas, the ultrasound tests returned average values of the ultrasound between a minimum value of 3050 m/s² and a maximum value of 3660 m/s². Comparing the results by using the method SonReb, the obtained values of the concrete resistance are from a minimum value of 18 MPa to a maximum value of 22 MPa, that take in a significant consideration the contribution of the covered concrete conditions.


## 4.1. On-Site Tests: Formulation

Essential elements for the organisation of an investigation campaign are the selection of the components that will be examined (which have to be representative of the whole structure), the investigation methodology that will be used, and the number and location of the investigation points; these requirements, in fact, are fundamental to guarantee a certain level of “reliability” of the obtained results and a “trustworthiness” with regard to the qualitative indications related to the characteristics of the material. In the case of the “Centrone” theatre, the identification of the components to be investigated was made by selecting the structural components which make the internal core of the load-bearing structure for two reasons: (1) because they enable to investigate a concrete in the state of “natural aging” (i.e., without considering the aggressive atmospheric agents which could have modified the condition of the material) and (2) for easiness of selecting the testing points. The structure of the whole building consists of a dual typology of structural components: those inserted in the external fabric (therefore difficult to investigate) and those located within the building.The selection of the location of the investigation points (Figure8) was random (with the aim to guarantee the representativeness of the investigation for the entire structure); in addition, “homogenous” areas [1] (which have the same characteristics) were noted and considered by making the obtained results “qualitative” and representative for all the components that show the same characteristics; a further condition is that the selected surfaces do not show any obvious condition of degradation. The methodology used to undertake the tests was exclusively selected in terms of the possibility to undertake the tests. Regarding the sclerometric tests, they were undertaken by placing the instrument always orthogonally in relation to the investigated surface; the preference was given to the direct method of investigation.The considered reference (in terms of the number of tests with the aim to guarantee the reliability of the results) for the investigation campaign was taken from the framework of the Italian investigation procedures.Figure 8
The specification of the location of the investigation points.


## 4.2. On-Site Tests: Analysis and Results

Sclerometer tests were carried out following the directions contained in UNI EN 12504-2 (2001). The instrument used is the concrete GEI model. On each pillar identified, it was carried out 10 measurements (Table1) of the value of rebound (for each test, ten values were taken, from which the average value was considered as illustrative).Table 1
The value of rebound index.
Structural element
Sclerometer value
Average value
Element code
Size [cm]
Rebound value
P1 Dx  T
43 × 43
27
28
26
29
25
25
31
26
28
28
28
P2 Dx   T
43 × 43
34
38
36
42
40
36
37
38
41
38
38
P3 Dx   T
43 × 43
32
33
30
31
32
32
34
31
31
31
32
P4 Dx   T
43 × 43
35
33
34
30
36
34
34
34
36
38
38
P5 Dx   T
43 × 43
35
33
34
34
33
32
35
37
34
34
34
P6 Dx   T
43 × 43
35
37
38
38
36
34
35
38
36
36
36
P1 Sx  T
43 × 43
41
37
45
47
37
38
42
39
40
41
41
P2 Sx  T
43 × 43
43
42
42
40
44
42
46
44
44
40
43
P3 Sx  T
43 × 43
34
34
37
35
34
33
34
32
36
35
34
P4 Sx T
43 × 43
32
28
32
32
34
34
34
34
30
32
32
P5 Sx   T
43 × 43
30
28
28
32
30
28
32
32
30
30
30
P6 Sx  T
43 × 43
34
35
34
36
35
37
38
35
38
35
36
P1 Dx   I p
43 × 43
23
21
21
22
22
25
25
26
24
22
23
P2 Dx   I p
43 × 43
33
32
33
32
30
30
30
33
31
30
31
P3 Dx  I p
43 × 43
37
40
38
41
43
38
38
38
41
38
39
P4 Dx   I p
43 × 43
38
38
38
38
37
39
37
38
39
39
38
P5 Dx   I p
43 × 43
37
39
35
38
37
38
38
40
38
40
38
P6 Dx   I p
43 × 43
36
38
37
37
38
38
37
38
36
38
37
P1 Sx  I p
43 × 43
26
22
24
22
24
20
23
22
22
22
23
P2 Sx  I p
43 × 43
40
41
37
40
40
39
38
38
37
38
39
P3 Sx  I p
43 × 43
40
37
35
37
36
35
35
35
35
35
36
P4 Sx  I p
43 × 43
35
35
35
37
35
37
36
38
36
38
36
P5 Sx  I p
43 × 43
40
40
37
35
36
35
38
36
36
36
37
P6 Sx  I p
43 × 43
36
38
36
38
38
38
40
40
38
38
38Three different areas were selected for each investigated component; at 0.70 m, at 1.40 m, and at 2.10 m from the floor. This selection, in fact, was motivated by the need to investigate the columns at the points of major stress (base and middle), having assumed (1) a uniform distribution of the loads and imposed loads (due to the homogenous structure) and (2) a homogenous condition of the loads (there are no visible cracks to induce any different considerations).Ultrasonic tests were carried out according to the UNI EN 12504-4 (2005). Ultrasonic equipment used is the DSP model of Ultrasonic UTD 1004. On each pillar identified, it was carried out 10 measurements (Table2) of the value of rebound (for each test ten values were taken, from which the average value was considered as illustrative).Table 2
The value of ultrasonic speed.
P1 Sx T average ultrasonic speed: 2862,9 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2039
2036
2035
2038
2041
2032
2034
2045
2048
2029
Y direction
3656
3669
3686
3676
3664
3668
3672
3675
3663
3665
Height: 1,40 mSize 0,43 × 0,43
X direction
2043
2041
2042
2045
2046
2049
2068
2061
2043
2048
Y direction
3665
3681
3687
3690
3684
3689
3676
3679
3695
3700
Height: 2,10 mSize 0,40 × 0,40
X direction
2052
2045
2049
2046
2048
2058
2060
2039
2059
2056
Y direction
3685
3684
3682
3679
3669
3689
3694
3692
3686
3696
P1 Dx  T average ultrasonic speed: 2873,2 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
3367
3355
3362
3360
3355
3394
3397
3389
3362
3392
Y direction
2520
2521
2531
2513
2512
2515
2510
2533
2511
2525
Height: 1,40 mSize 0,43 × 0,43
X direction
3250
3257
3260
3252
3247
3302
3315
3333
3341
3348
Y direction
2490
2499
2510
2512
2505
2496
2493
2495
2491
2510
Height: 2,10 mSize 0,40 × 0,40
X direction
3322
3320
3333
3327
3325
3139
3152
3134
3152
3157
Y direction
2526
2516
2545
2544
2558
2556
2559
2562
2568
2564
P6 Sx  T average ultrasonic speed: 2134,1 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2160
2084
2053
2016
2066
2161
2016
2103
2105
2150
Y direction
2160
2154
2111
2102
2013
2163
2136
2165
2130
2122
Height: 1,40 mSize 0,43 × 0,43
X direction
2160
2136
2165
2154
2155
2155
2153
2151
2160
2165
Y direction
2152
2154
2150
2153
2103
2100
2155
2015
2140
2150
Height: 2,10 mSize 0,40 × 0,40
X direction
2150
2099
2088
2066
2200
2035
2150
2156
2171
2015
Y direction
2030
2105
2145
2144
2014
2156
2148
2154
2148
2154
P6 Dx  T average ultrasonic speed: 2560,9 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
2562
2563
2545
2568
2567
2575
2574
2586
2544
2578
Y direction
2543
2546
2566
2564
2568
2545
2544
2543
2549
2548
Height: 1,40 mSize 0,43 × 0,43
X direction
2566
2531
2533
2540
2545
2562
2545
2565
2555
2551
Y direction
2556
2565
2559
2557
2549
2552
2553
2545
2551
2553
Height: 2,10 mSize 0,40 × 0,40
X direction
2565
2596
2586
2567
2568
2564
2572
2575
2574
2573
Y direction
2564
2561
2563
2559
2568
2567
2586
2584
2583
2569
P1 Sx  I p average ultrasonic speed: 2582,0 m/s
Height: 0,70 mSize 0,46 × 0,46
X direction
1899
2130
2156
2102
2105
2111
2182
2221
2310
2229
Y direction
3200
3180
3196
3102
3104
3016
3038
3086
3048
3062
Height: 1,40 mSize 0,43 × 0,43
X direction
1700
1750
1890
1806
1830
1834
1905
1942
1972
1973
Y direction
3109
3140
3149
3131
3158
3160
3263
3264
3285
3189
Height: 2,10 mSize 0,40 × 0,40
X direction
2005
2103
1999
2150
2015
2060
2160
2163
2184
2150
Y direction
3005
3158
3139
3190
3100
3089
3048
3069
3099
3105
P1 Dx  I p average ultrasonic speed: 3006,5 m/s
Height: 0,70 mSize 0,46 ×  0,46
X direction
3000
3002
3005
3019
2993
3010
3015
3019
2921
2996
Y direction
3012
3015
3018
3016
3018
3001
3021
3029
3028
3020
Height: 1,40 mSize 0,43 ×  0,43
X direction
3000
3052
3013
3002
3015
2999
3050
3015
3016
3019
Y direction
2996
3047
3036
3033
3031
3002
3052
3035
3063
3043
Height: 2,10 mSize 0,40 ×  0,40
X direction
2899
2915
3005
3001
3045
3015
3062
3036
3035
3046
Y direction
3051
3015
3063
3026
3033
3018
3017
3021
3012
3026These data were compared with the method “SonReb” (Tables3, 4, 5, and 6) to improve—as said before—the qualitative interpretation of results; the analysis showed satisfactory results of the state of concrete condition, as well as the importance to compare the ultrasonic and sclerometer tests.Table 3
Left side pillar (Sx): Ground floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Sx T
41
2862,9
P2 Sx T
43
3297,1
P3 Sx T
34
3345,3
P4 Sx T
32
3181,2
P5 Sx T
30
3192,1
P6 Sx T
36
2134,1Table 4
Right side pillar (Dx): Ground floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Dx T
28
2873,2
P2 Dx T
38
3103,6
P3 Dx T
32
3199,3
P4 Dx T
38
3313,2
P5 Dx T
34
3082,1
P6 Dx T
36
2560,9Table 5
Left side pillar (Sx): First floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Sx I p
23
2582,0
P2 Sx I p
39
3476,1
P3 Sx I p
36
3358,2
P4 Sx I p
36
3319,6
P5 Sx I p
37
3450,3
P6 Sx I p
38
3346,1Table 6
Right side pillar (Dx): First floor.
Pillar
Average rebound value
Average ultrasonic speed
P1 Dx I p
23
3006,5
P2 Dx I p
31
3210,2
P3 Dx I p
39
3120,9
P4 Dx I p
38
3204,6
P5 Dx I p
38
3098,1
P6 Dx I p
37
3301,5The obtained results show a significant homogeneity of values measured at each investigated level; more precisely, the sclerometric tests show an average value (of the ten measurements made at each point) of the bounce index uniformly distributed on the surfaces; whereas, the ultrasound tests returned average values of the ultrasound between a minimum value of 3050 m/s² and a maximum value of 3660 m/s². Comparing the results by using the method SonReb, the obtained values of the concrete resistance are from a minimum value of 18 MPa to a maximum value of 22 MPa, that take in a significant consideration the contribution of the covered concrete conditions.


## 5. Conclusions

The tests carried out are the basis of a diagnostic project that is possible to implement and monitor to guarantee a deeper knowledge, with the goal of attaining a level of thorough understanding aimed at the “preservation and improvement” of a building.The recovery project, that takes particular care in the methodological application of the diagnostic phase, cannot leave out of consideration the necessity of a careful and timely monitoring of building conditions.The carried out tests are the first and simplest analysis for a qualitative assessment; it is necessary to classify the structure regarding the following consolidation procedures. The recovery and conservation project, as well as an “indispensable” transformation of an old building, must be in that evaluations, of feasibility and suitability, both economic and practice which is the basis for a “suitable choice” of recovery intervention, that permit to annul the “cancellation” of the Built Heritage.



---

*Source: 659612-2012-09-27.xml*